comparisonofdifferentcharacteristics of modern … · c si mn p s cr mo v co cr/c mo/c v/c 1.2343...
Embed Size (px)
COMPARISON OF DIFFERENT CHARACTERISTICSOF MODERN HOT-WORK TOOL STEELS
P. GumpelFachhochschule Konstanz (University of Applied Sciences),
T. BogatzkyInstitute fur Werkstoffsystemtechnik Thurgau an der Fachhochschule Konstanz,
Konstanzer Strasse 19,
A. Huber and B. GeiggesAlusuisse Singen GmbH,
Hot-work tool steels in operation are subjected to distinctmechanicalforces and considerable changes in temperature. The complex effects ofmechanical, thermal, and chemical factors on the tools in operation implydemanding requirements for hot-work tool steels. In recentyears a number ofinvestigations have been made as tohow different alloying elements affect thematerial properties of hot-work tool steels [1, 2, 3]. Basedon more profoundknowledge in this field, new materials were developed and brought to marketso that nowadays users have a wide range of material grades with differencesin quality to choose from. In addition to changes in the composition of alloysa variety of processing techniques may also influence material quality [4, 5].
4 6TH INTERNATIONAL TOOLING CONFERENCE
Application of carefully directed forming and tempering operations mayresult in specific material characteristics like isotropy of mechanical prop-erties, formation of structure, as well as content, shape and distribution ofnon-metallic inclusions. Thus users face a great number of alternative mate-rials to choose from. The material assessment for extrusiontools will serveas an example of a procedure for the systematic selection of the most suitablematerial and an investigation is to be made into the differences in qualitybetween the respective materials. From a number of materials suitable forthis purpose, disks of the same dimensional category were procured andsubjected to tests relevant to the service life to be expected.
For the investigation disks were procured from round bars ofthe respec-tive steels, the dimensions were 320 mm in diameter, 30 mm thickness, thecondition was soft annealed. The steels were grade 1.2343 and 1.2367 aswell as three special grades, designated Special A, B, and C.The soft an-nealed samples were pickled to establish the degree of segregation in thematerials, and in addition to that the annealed structure inthe transversedirection was determined, shown in Fig. 1. For the testing ofmechanicalproperties specimens for notched bar impact test, impact bending test, andtensile test to destruction were taken from the transitional area of the disksin a transverse orientation. Each of the sample blanks was tempered at thecompany producing that particular steel grade. Additionaldata as far as theyare relevant for assessing the test results are presented together with theseresults.
The analysis of each of the supplied steel samples established its chemicalcomposition as shown in Table 1. From the results of the analyses theratios chromium /carbon, molybdenum/carbon, and vanadium/carbon werecalculated and included in the table. The results indicate that Special Aas well as Special C are variants of the original steel grade 1.2343 withlowered carbon content and simultaneously increased vanadium content.Hence there is a considerable change of the chromium/carbonratio as wellas a significantly changed vanadium/carbon ratio. Both changes are due
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 5
to recommendations made after earlier tests, to change the ratio of carbideformers to carbon content in this steel [2, 3]. In the alloying variant Special Athe molybdenum content is also higher than in 2343. Special Bis a variant ofsteel 1.2367 resulting from an additional alloying of a higher cobalt content.
Table 1. Analyses of tested materials as measured
Designation Composition of material Ratio of carbide formersto carbon content
C Si Mn P S Cr Mo V Co Cr/ C Mo/ C V/ C
1.2343 0.369 0.882 0.398 0.012 0.005 4.37 1.14 0.28 0.01 11.84 3.09 0.761.2367 0.374 0.335 0.327 0.017 0.004 4.37 3.07 0.55 < 0,01 11.68 8.21 1.47Special A 0.345 0.38 0.331 0.015 0.006 4.74 1.96 0.56 < 0,01 13.74 5.68 1.62Special B 0.355 0.39 0.35 0.026 0.005 4.22 2.89 0.5 2.58 11.898.14 1.41Special C 0.321 0.308 0.24 0.019 0.005 4.33 1.27 0.41 < 0,01 13.49 3.96 1.28
The pickling test makes existing block segregations visible. If segrega-tions exist, the chemicals affect the material more or less strongly dependingon their respective alloying composition, and the resulting effect becomesnoticeable with changing surface brightness. The ground specimens werepickled as follows: 50% H2O plus 50% HCl (mixed to 37% content) at roomtemperature for 40minutes. During this test no differenceswere visible in thedegree of segregations in the materials. All disks showed a macroscopicallyhomogeneous distribution of alloying elements across the entire surface.
The annealed structure was classified as suggested by the North AmericanDie Casting Association (NADCA). Accordingly, steel grade1.2343 wasclassified D1. This means it is acceptable, the carbide distribution, how-ever, is not homogeneous. There are regions containing significantly fewercarbides. Moreover, string-like structures are apparent.The annealed struc-ture of steel 1.2367 was classified B2 according to NADCA. Theannealedstructure shows a fine distribution of carbides, but they arenot distributed ho-mogeneously, as can be seen from slight difference in contrast Fig. 1b. Theannealed structure of Special A was classified NADCA A1, which is equiv-
6 6TH INTERNATIONAL TOOLING CONFERENCE
alent to very good. Carbide distribution in Special B is somewhat coarser,that meant NADCA classification B1 in this case. Carbides in Special Care comparatively fine but have not been completely formed. Moreover, aslight irregularity of carbide distribution is evident from a needle-like ma-trix. The annealed structure of this steel was classified B1 –C1 accordingto NADCA. All annealed structures were studied and classified accordingto NADCA guidelines for longitudinal as well as transverse specimens, andthe results have been compiled in Table 2.
Table 2. Results of structure classification according to NADCA guidelines
Annealed structure according to NADCA
Steel Longitudinal sample Transversal Sample
1.2343 D1 D11.2367 B2 A3Special A A1 A1Special B B1 B1Special C C1 B1
HEAT TREATMENT AND TEMPERED STRUCTURE
The structures observed in heat-treated samples are presented in Fig. 2together with the parameters of heat treatment and final hardness measured.Already at first sight, pronounced differences are obvious.Material 1.2343quenched from a temperature of 1010◦Chas a coarse grain with coarse,needle-like martensite structure. The other materials hardly differ from oneanother, for example Special C has the smallest austenite grain size. Thissteel was, however, hardenedat the lowest austenitizing temperature. If hard-ness is compared after the last tempering process, which wasat 570◦Cforall steels, the low-carbon steel variants show significantly higher temperingthan the original steel 1.2343. The result corresponds to findings presentedin other publications , according to which variants of hot-work tool steelX 40 Cr MoV 51 with lower carbon content have a lower secondaryhardness,and in the technically important range of tempering temperatures these low-
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 7
carbon steels have almost identical and occasionally even higher hardnessthan higher-carbon steels.
MECHANICAL, TECHNOLOGICAL PROPERTIES
All steels underwent tensile tests to destruction at room temperature, at450◦Cand at 550◦C. Figure 3 shows the tensile strengths of all steels tested.There is hardly any difference between the tensile strengths of each steel,and existing deviations nearly correspond to the differences in hardnessmeasured. As is to be expected, tensile strength and yield strength definitelydecrease at higher test temperatures. This decrease of strength is more orless strongly developed with each material, so that at high test temperatures,for example at 550◦C, the steels do show quite different results (Fig. 3).
Figure 4 presents the proportional decrease of tensile strength and yieldstrength and how they relate to the values at room temperature. It is obviousthat above all Special A and Special C demonstrate a very favorable behavior.Tensile strength at room temperature as well as at raised temperatures de-pends on precipitated carbon content as well as on dissolvedcarbon contentin the matrix. Both of these are influenced by the ratio of carbide formingelements to carbon in the steel. Therefore Fig. 5 shows tensile strength atdifferent temperatures and its dependence on the ratio chromium/carbon,vanadium/carbon and molybdenum/carbon. Here is an indication that par-ticularly with Special C a very favorable ratio of carbide formers to car-bon has been achieved. It becomes evident that neither an increase of theratio chromium/carbon nor one of the ratio vanadium/carbon, or molybde-num/carbon would be able to contribute to any further increase of tensilestrength. A similar observation as for steel grades 2343 cannot be madefor steel grades 2367 as the ratio chromium/carbon, molybdenum/carbon,and vanadium/carbon remained almost identical and only more cobalt wasalloyed to the steel. This higher cobalt content does not result in any im-provement of tensile strength at higher temperatures as canbe seen fromFig. 4 when comparing steel 1.2367 with Special B.
The toughness of the respective steels was tested in notchedrod impacttests and in impact bending tests. The notched rod impact tests were carriedout according to DIN 50 115 (German Industrial Standard) on V-notchedspecimens with a pendulum impact-testing machine with 450 Joule impactload at room temperature. The impact bending tests were carried out accord-ing to DIN 50 115 and DGM guidelines with the same pendulum impact-
8 6TH INTERNATIONAL TOOLING CONFERENCE
testing machine. The mean results of six tests each are summarized in Fig. 6.Here it becomes evident once again that Special C generally has the mostfavorable toughness. The least favorable results are foundwith steel 1.2367,whilst the almost identical steel with a higher cobalt content has significantlybetter toughness. Also with respect to toughness, certain observations can bemade about the influence of the ratio of carbide forming alloying elementsto carbon (Fig. 7). Once more, optimal results are achieved with SpecialC, having a ratio chromium/carbon of about 13.5, a ratio vanadium/carbonof about 1.3 and a ratio molybdenum/carbon of about 4. Surelythe statedinfluence of alloy composition can be further enhanced by different forg-ing and/or tempering procedures. An interesting finding in this context isthat with almost the same basic alloying compositions the ratio of carbideforming elements to carbon has such a very positive effect.
To enable a valid assessment of the overall properties of thesteels theindividual results were plotted on a radar chart (Fig. 8). The hardness andtensile strengths at 450◦Cand 550◦Creflect the strengths of the steels. Theimpact bending load, the notch impact load and the reductionof area at550◦Care indicators for the toughness of each steel. The larger the areaenclosed is, the better are the overall properties of the material. As wasalready to be concluded from the measured values, Special C has the largestenclosed area and thus exhibits the best overall properties. Special A alsoshows quite positive overall properties, whilst Special B has a less favorableresult than original grade 1.2343 everything being considered. For material1.2367 the results of this investigation were generally inadequate.
DISCUSSION OF TEST RESULTS
In order to improve the mechanical properties and in particular the tough-ness of hot-work tool steels there are two options of proceeding:
changing forging and heat treatment
changing the material.
Optimization of hot-work tool steels by alloying techniques as pursued bysteel producers appears to be a very promising option, considering the re-sults of this investigation. The ratio of carbide forming alloying elements tocarbon content offers a possibility to control above all thecarbide reactionin the steel. Carbon, chromium, molybdenum, and vanadium are respon-
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 9
sible for the formation of carbides in hot-work tool steels containing theseelements.
In the annealed condition the total carbon content of hot-work tool steelsis available in the form of carbides. In the course of hardening and temper-ing, a large portion of carbon is dissolved and stored in the matrix where itinfluences the transformation behavior noticeably. Decreasing carbon con-tent increases the Ms and Mf temperatures significantly, but its effect onAc1b and Ac1e temperatures is negligible. With a higher ratio of carbide for-mers to carbon there is less hardenability. Lower carbon steels have a lowersecondary hardness maximum . Previous investigations have shown thatfurther elevation of the tempering temperature, i.e. abovethe secondaryhardness maximum, reduces these differences again . As this levels offthe steep drop in hardness when annealing lower carbon steels, the requiredoperational hardness should be more easily achieved. In general, due tothe restricted availability of carbon, lower carbide contents are found in theannealed condition as well as in the tempered condition. Because of thislower carbide content, toughness is improved. It has repeatedly been shownin earlier investigations that by lowering the carbon content in hot-work toolsteels 1.2344 and 1.2343 hot-work strength, hot-work toughness, and creepstrength can be improved simultaneously. Those laboratorytests have beenconfirmed by this investigation of hot-work tool steels as produced by themill. At present the materials are being tested in the extrusion of aluminumsections. Operational results up to now suggest that the systematic selectionof material presented here will optimize the service time ofextrusion tools.
 P. GUMPEL, Einflußerhohter Chromgehalte auf die Eigenschaften des Warmar-beitsstahles X 38 Cr MoV 51. Thyssen Edelstahl Techn. Ber. 5 (1979) s.129/134.
 H. BERNS and F. WENDL, Effect of carbon content in Cr MoV hot working tool steel.steel research 57(12) (1986), s.671.
 A. DITTRICH, E. HABERLING, K. ROSCHE and I. SCHRUFF, Legierungsop-timierung des Warmarbeitsstahles X 40 Cr Mo V 51 (1.2344) fur großformatigeWerkzeuge mit hoher Zahigkeitsbeanspruchung. Thyssen Edelstahl Techn.Ber. 15(1989) s. 63.
 H. BERNS, E. HABERLING and F. Wendl, Einflußdes Gluhgefuges auf die Zahigkeitvon Warmarbeits-stahlen. Thyssen Edelstahl Techn. Ber. 11 (1985) s. 150.
10 6TH INTERNATIONAL TOOLING CONFERENCE
 H. J. BECKER, H. BRANDIS, P. GUMPEL and E. HABERLING, Stand und En-twicklungstendenzen auf dem Gebiet der Werkzeugstahle Stahl und Eisen 105 (1985)s. 257/65.
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 11
(a) 1.2343 (b) 1.2367
(c) Special A (d) Special B
(e) Special C
Figure 1. Annealed microstructure of cross-sections of transverse cuts in the transitionalregion.
12 6TH INTERNATIONAL TOOLING CONFERENCE
(a) 42 HRC, 1.23431010◦C/ 45 min/ Polymer620◦C/ 610◦C/ 570◦C
(b) 44 HRC, 1.23671030◦C/ 45 min/ Polymer640◦C/ 610◦C/ 570◦C
(c) 43 HRC, Special A1010◦C/ 45 min/ Polymer640◦C/ 580◦C/ 570◦C
(d) 42,5 HRC, Special B1030◦C/ 45 min/ Polymer640◦C/ 580◦C/ 570◦C
(e) 44 HRC, Special C , 1000◦C/ 45 min/Ol625◦C/ 580◦C/ 570◦C
Figure 2. Hardened and annealed structure of tested steels with data on heat treatment andfinal hardness measured HRC.
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 13
Figure 3. Survey of tensile strength values established in tensile tests at room temperatureand at elevated temeratures.
Figure 4. Drop of tensile strength at elevated temperatures as compared to tensil strengthat room temperature.
14 6TH INTERNATIONAL TOOLING CONFERENCE
Figure 5. Effect of the ratio of carbide forming elements to carbon on material strengthproperties, based on steel grade 1.2343.
Comparison of Different Characteristics of Modern Hot-Work Tool Steels 15
Figure 6. Toughness comparison of tested steels.
Figure 7. Influence of the ratio of carbide forming elements to carbon on toughness, basedon steel grade 1.2343.
16 6TH INTERNATIONAL TOOLING CONFERENCE
Figure 8. Assessment of the overall properties of tested steels.